# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2024

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_BaYZnSiO
_audit_block_doi                 10.25505/fiz.icsd.cc2fz7xl
_database_code_depnum_ccdc_archive 'CCDC 2263400'
loop_
_audit_author_name
_audit_author_address
ahmetjan
;ucas
China
;
_audit_update_record             
;
2023-05-16 deposited with the CCDC.	2024-01-17 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Ba5 O40 Si8 Y12 Zn'
_chemical_formula_weight         2683.71

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      tetragonal
_space_group_IT_number           121
_space_group_name_H-M_alt        'I -4 2 m'
_space_group_name_Hall           'I -4 2'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'y, -x, -z'
'-x, -y, z'
'-y, x, -z'
'x, -y, -z'
'-y, -x, z'
'-x, y, -z'
'y, x, z'
'x+1/2, y+1/2, z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'y+1/2, x+1/2, z+1/2'

_cell_length_a                   18.7014(6)
_cell_length_b                   18.7014(6)
_cell_length_c                   5.3640(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     1876.02(14)
_cell_formula_units_Z            2
_cell_measurement_temperature    273(2)
_cell_measurement_reflns_used    5747
_cell_measurement_theta_min      3.95
_cell_measurement_theta_max      27.40

_exptl_crystal_description       Block
_exptl_crystal_colour            Colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.751
_exptl_crystal_F_000             2420
_exptl_transmission_factor_min   0.07851
_exptl_transmission_factor_max   0.18676
_exptl_crystal_size_max          0.143
_exptl_crystal_size_mid          0.130
_exptl_crystal_size_min          0.094
_exptl_absorpt_coefficient_mu    24.466
_shelx_estimated_absorpt_T_min   0.0400
_shelx_estimated_absorpt_T_max   0.5285
_exptl_absorpt_correction_type   Numerical
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   Face-index
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      273(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            12254
_diffrn_reflns_av_unetI/netI     0.0363
_diffrn_reflns_av_R_equivalents  0.0720
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_theta_min         1.540
_diffrn_reflns_theta_max         27.466
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measured_fraction_theta_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_point_group_measured_fraction_full 0.997
_reflns_number_total             1122
_reflns_number_gt                1081
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.710
_reflns_Friedel_fraction_max     0.998
_reflns_Friedel_fraction_full    0.997

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0197P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_extinction_coef       0.00075(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 
;
 Flack x determined using 430 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   -0.007(6)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         1122
_refine_ls_number_parameters     85
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0224
_refine_ls_R_factor_gt           0.0212
_refine_ls_wR_factor_ref         0.0471
_refine_ls_wR_factor_gt          0.0468
_refine_ls_goodness_of_fit_ref   1.013
_refine_ls_restrained_S_all      1.013
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1 Ba 1.000000 0.83930(3) 1.000000 0.01109(16) Uani 1 2 d S T P . .
Ba2 Ba 0.500000 1.000000 0.750000 0.0290(5) Uani 0.5 4 d S T P . .
Y1 Y 0.79158(3) 0.79158(3) 0.00488(18) 0.0076(2) Uani 1 2 d S T P . .
Y2 Y 0.68727(4) 0.89941(4) 0.44909(13) 0.00746(17) Uani 1 1 d . . . . .
Zn1 Zn 1.000000 1.000000 0.500000 0.0137(5) Uani 1 8 d S T P . .
Si1 Si 0.87484(11) 0.87484(11) 0.4412(5) 0.0085(6) Uani 1 2 d S T P . .
Si2 Si 0.65819(14) 1.000000 0.000000 0.0087(5) Uani 1 2 d S T P . .
O1 O 0.9336(3) 0.9336(3) 0.3341(15) 0.0117(17) Uani 1 2 d S T P . .
O2 O 0.8141(3) 0.7044(3) -0.2722(10) 0.0088(11) Uani 1 1 d . . . . .
O3 O 0.8703(3) 0.8703(3) 0.7422(14) 0.0129(17) Uani 1 2 d S T P . .
O4 O 0.7070(3) 1.0172(3) 0.2434(9) 0.0087(12) Uani 1 1 d . . . . .
O5 O 0.6119(3) 0.9305(3) 0.0865(10) 0.0132(12) Uani 1 1 d . . . . .
O6 O 0.7992(3) 0.8936(3) 0.3024(10) 0.0106(11) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1 O6 2.674(5) 8_556 ?
Ba1 O6 2.674(5) 4_756 ?
Ba1 O1 2.804(5) 1_556 ?
Ba1 O1 2.804(5) 4_756 ?
Ba1 O4 2.817(5) 4_756 ?
Ba1 O4 2.817(5) 8_556 ?
Ba1 O3 2.852(5) . ?
Ba1 O3 2.852(5) 4_757 ?
Ba1 Si2 3.387(3) 4_756 ?
Ba1 Si1 3.394(2) 1_556 ?
Ba1 Si1 3.394(2) 4_756 ?
Ba1 Y1 3.9988(8) 1_556 ?
Ba2 O5 2.614(5) 5_576 ?
Ba2 O5 2.614(5) 7_656 ?
Ba2 O5 2.614(5) 14_665 ?
Ba2 O5 2.614(5) 16_455 ?
Ba2 Ba2 2.68200(10) 5_576 ?
Ba2 Ba2 2.68200(11) 5_577 ?
Ba2 O5 3.053(5) 10_465 ?
Ba2 O5 3.053(6) 1_556 ?
Ba2 O5 3.053(5) 12_655 ?
Ba2 O5 3.053(6) 3_676 ?
Ba2 Si2 3.248(2) 10_465 ?
Ba2 Si2 3.248(2) 1_556 ?
Y1 O2 2.246(6) 8 ?
Y1 O2 2.246(5) . ?
Y1 O2 2.311(5) 14_665 ?
Y1 O2 2.311(5) 11_665 ?
Y1 O6 2.492(6) 8 ?
Y1 O6 2.492(6) . ?
Y1 O3 2.514(8) 1_554 ?
Y1 Si1 3.213(3) . ?
Y1 Y1 3.4684(11) 11_664 ?
Y1 Y1 3.4684(11) 11_665 ?
Y1 Y2 3.6060(9) 11_664 ?
Y1 Y2 3.6060(9) 14_664 ?
Y2 O2 2.210(5) 8_556 ?
Y2 O6 2.238(5) . ?
Y2 O2 2.276(5) 11_665 ?
Y2 O4 2.300(5) 5_576 ?
Y2 O5 2.332(5) 14_665 ?
Y2 O5 2.472(6) . ?
Y2 O4 2.490(5) . ?
Y2 Si2 3.1044(9) . ?
Y2 Y2 3.5283(9) 14_664 ?
Y2 Y2 3.5283(9) 14_665 ?
Zn1 O1 1.970(7) 3_775 ?
Zn1 O1 1.970(7) 2_576 ?
Zn1 O1 1.970(7) 4_756 ?
Zn1 O1 1.970(7) . ?
Si1 O3 1.619(8) . ?
Si1 O6 1.637(6) 8 ?
Si1 O6 1.637(6) . ?
Si1 O1 1.656(8) . ?
Si2 O4 1.624(5) . ?
Si2 O4 1.624(5) 5_575 ?
Si2 O5 1.630(6) 5_575 ?
Si2 O5 1.630(6) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 Ba1 O6 147.4(2) 8_556 4_756 ?
O6 Ba1 O1 57.25(19) 8_556 1_556 ?
O6 Ba1 O1 153.3(2) 4_756 1_556 ?
O6 Ba1 O1 153.3(2) 8_556 4_756 ?
O6 Ba1 O1 57.25(19) 4_756 4_756 ?
O1 Ba1 O1 102.1(3) 1_556 4_756 ?
O6 Ba1 O4 87.12(15) 8_556 4_756 ?
O6 Ba1 O4 63.71(15) 4_756 4_756 ?
O1 Ba1 O4 142.95(18) 1_556 4_756 ?
O1 Ba1 O4 107.86(18) 4_756 4_756 ?
O6 Ba1 O4 63.71(15) 8_556 8_556 ?
O6 Ba1 O4 87.12(15) 4_756 8_556 ?
O1 Ba1 O4 107.86(18) 1_556 8_556 ?
O1 Ba1 O4 142.95(18) 4_756 8_556 ?
O4 Ba1 O4 57.0(2) 4_756 8_556 ?
O6 Ba1 O3 73.6(2) 8_556 . ?
O6 Ba1 O3 113.30(19) 4_756 . ?
O1 Ba1 O3 78.77(17) 1_556 . ?
O1 Ba1 O3 86.5(2) 4_756 . ?
O4 Ba1 O3 81.78(16) 4_756 . ?
O4 Ba1 O3 120.02(19) 8_556 . ?
O6 Ba1 O3 113.30(19) 8_556 4_757 ?
O6 Ba1 O3 73.6(2) 4_756 4_757 ?
O1 Ba1 O3 86.5(2) 1_556 4_757 ?
O1 Ba1 O3 78.77(17) 4_756 4_757 ?
O4 Ba1 O3 120.02(19) 4_756 4_757 ?
O4 Ba1 O3 81.78(16) 8_556 4_757 ?
O3 Ba1 O3 156.5(3) . 4_757 ?
O6 Ba1 Si2 73.70(11) 8_556 4_756 ?
O6 Ba1 Si2 73.70(11) 4_756 4_756 ?
O1 Ba1 Si2 128.95(15) 1_556 4_756 ?
O1 Ba1 Si2 128.95(15) 4_756 4_756 ?
O4 Ba1 Si2 28.51(10) 4_756 4_756 ?
O4 Ba1 Si2 28.51(10) 8_556 4_756 ?
O3 Ba1 Si2 101.73(14) . 4_756 ?
O3 Ba1 Si2 101.73(14) 4_757 4_756 ?
O6 Ba1 Si1 28.24(12) 8_556 1_556 ?
O6 Ba1 Si1 172.24(12) 4_756 1_556 ?
O1 Ba1 Si1 29.04(16) 1_556 1_556 ?
O1 Ba1 Si1 128.91(16) 4_756 1_556 ?
O4 Ba1 Si1 114.62(11) 4_756 1_556 ?
O4 Ba1 Si1 85.84(11) 8_556 1_556 ?
O3 Ba1 Si1 73.24(15) . 1_556 ?
O3 Ba1 Si1 102.05(17) 4_757 1_556 ?
Si2 Ba1 Si1 101.29(4) 4_756 1_556 ?
O6 Ba1 Si1 172.24(12) 8_556 4_756 ?
O6 Ba1 Si1 28.24(12) 4_756 4_756 ?
O1 Ba1 Si1 128.91(16) 1_556 4_756 ?
O1 Ba1 Si1 29.04(16) 4_756 4_756 ?
O4 Ba1 Si1 85.84(11) 4_756 4_756 ?
O4 Ba1 Si1 114.62(11) 8_556 4_756 ?
O3 Ba1 Si1 102.05(16) . 4_756 ?
O3 Ba1 Si1 73.24(15) 4_757 4_756 ?
Si2 Ba1 Si1 101.29(4) 4_756 4_756 ?
Si1 Ba1 Si1 157.42(8) 1_556 4_756 ?
O6 Ba1 Y1 37.66(12) 8_556 1_556 ?
O6 Ba1 Y1 131.79(12) 4_756 1_556 ?
O1 Ba1 Y1 72.79(14) 1_556 1_556 ?
O1 Ba1 Y1 125.20(13) 4_756 1_556 ?
O4 Ba1 Y1 72.29(10) 4_756 1_556 ?
O4 Ba1 Y1 84.95(10) 8_556 1_556 ?
O3 Ba1 Y1 38.68(17) . 1_556 ?
O3 Ba1 Y1 150.61(14) 4_757 1_556 ?
Si2 Ba1 Y1 77.103(10) 4_756 1_556 ?
Si1 Ba1 Y1 50.72(5) 1_556 1_556 ?
Si1 Ba1 Y1 136.09(4) 4_756 1_556 ?
O5 Ba2 O5 140.8(2) 5_576 7_656 ?
O5 Ba2 O5 96.46(8) 5_576 14_665 ?
O5 Ba2 O5 96.46(8) 7_656 14_665 ?
O5 Ba2 O5 96.46(8) 5_576 16_455 ?
O5 Ba2 O5 96.46(8) 7_656 16_455 ?
O5 Ba2 O5 140.8(2) 14_665 16_455 ?
O5 Ba2 Ba2 109.60(12) 5_576 5_576 ?
O5 Ba2 Ba2 109.60(12) 7_656 5_576 ?
O5 Ba2 Ba2 70.40(12) 14_665 5_576 ?
O5 Ba2 Ba2 70.40(12) 16_455 5_576 ?
O5 Ba2 Ba2 70.40(12) 5_576 5_577 ?
O5 Ba2 Ba2 70.40(12) 7_656 5_577 ?
O5 Ba2 Ba2 109.60(12) 14_665 5_577 ?
O5 Ba2 Ba2 109.60(12) 16_455 5_577 ?
Ba2 Ba2 Ba2 180.0 5_576 5_577 ?
O5 Ba2 O5 151.6(2) 5_576 10_465 ?
O5 Ba2 O5 61.12(13) 7_656 10_465 ?
O5 Ba2 O5 57.7(2) 14_665 10_465 ?
O5 Ba2 O5 97.95(19) 16_455 10_465 ?
Ba2 Ba2 O5 53.76(10) 5_576 10_465 ?
Ba2 Ba2 O5 126.24(10) 5_577 10_465 ?
O5 Ba2 O5 57.7(2) 5_576 1_556 ?
O5 Ba2 O5 97.95(19) 7_656 1_556 ?
O5 Ba2 O5 61.12(13) 14_665 1_556 ?
O5 Ba2 O5 151.6(2) 16_455 1_556 ?
Ba2 Ba2 O5 126.24(10) 5_576 1_556 ?
Ba2 Ba2 O5 53.76(10) 5_577 1_556 ?
O5 Ba2 O5 110.45(10) 10_465 1_556 ?
O5 Ba2 O5 61.12(13) 5_576 12_655 ?
O5 Ba2 O5 151.6(2) 7_656 12_655 ?
O5 Ba2 O5 97.95(19) 14_665 12_655 ?
O5 Ba2 O5 57.7(2) 16_455 12_655 ?
Ba2 Ba2 O5 53.76(10) 5_576 12_655 ?
Ba2 Ba2 O5 126.24(10) 5_577 12_655 ?
O5 Ba2 O5 107.5(2) 10_465 12_655 ?
O5 Ba2 O5 110.45(10) 1_556 12_655 ?
O5 Ba2 O5 97.95(19) 5_576 3_676 ?
O5 Ba2 O5 57.7(2) 7_656 3_676 ?
O5 Ba2 O5 151.6(2) 14_665 3_676 ?
O5 Ba2 O5 61.12(13) 16_455 3_676 ?
Ba2 Ba2 O5 126.24(10) 5_576 3_676 ?
Ba2 Ba2 O5 53.76(10) 5_577 3_676 ?
O5 Ba2 O5 110.45(10) 10_465 3_676 ?
O5 Ba2 O5 107.5(2) 1_556 3_676 ?
O5 Ba2 O5 110.45(10) 12_655 3_676 ?
O5 Ba2 Si2 126.25(12) 5_576 10_465 ?
O5 Ba2 Si2 71.68(12) 7_656 10_465 ?
O5 Ba2 Si2 29.86(12) 14_665 10_465 ?
O5 Ba2 Si2 126.18(12) 16_455 10_465 ?
Ba2 Ba2 Si2 65.62(2) 5_576 10_465 ?
Ba2 Ba2 Si2 114.38(2) 5_577 10_465 ?
O5 Ba2 Si2 29.77(10) 10_465 10_465 ?
O5 Ba2 Si2 81.74(10) 1_556 10_465 ?
O5 Ba2 Si2 112.33(10) 12_655 10_465 ?
O5 Ba2 Si2 129.18(10) 3_676 10_465 ?
O5 Ba2 Si2 29.86(12) 5_576 1_556 ?
O5 Ba2 Si2 126.18(12) 7_656 1_556 ?
O5 Ba2 Si2 71.68(12) 14_665 1_556 ?
O5 Ba2 Si2 126.25(12) 16_455 1_556 ?
Ba2 Ba2 Si2 114.38(2) 5_576 1_556 ?
Ba2 Ba2 Si2 65.62(2) 5_577 1_556 ?
O5 Ba2 Si2 129.18(10) 10_465 1_556 ?
O5 Ba2 Si2 29.77(10) 1_556 1_556 ?
O5 Ba2 Si2 81.74(10) 12_655 1_556 ?
O5 Ba2 Si2 112.33(10) 3_676 1_556 ?
Si2 Ba2 Si2 99.814(15) 10_465 1_556 ?
O2 Y1 O2 80.5(3) 8 . ?
O2 Y1 O2 121.76(10) 8 14_665 ?
O2 Y1 O2 73.48(13) . 14_665 ?
O2 Y1 O2 73.48(13) 8 11_665 ?
O2 Y1 O2 121.76(10) . 11_665 ?
O2 Y1 O2 77.7(3) 14_665 11_665 ?
O2 Y1 O6 165.71(19) 8 8 ?
O2 Y1 O6 108.76(17) . 8 ?
O2 Y1 O6 72.09(17) 14_665 8 ?
O2 Y1 O6 108.76(17) 11_665 8 ?
O2 Y1 O6 108.76(17) 8 . ?
O2 Y1 O6 165.72(19) . . ?
O2 Y1 O6 108.76(17) 14_665 . ?
O2 Y1 O6 72.09(17) 11_665 . ?
O6 Y1 O6 60.2(2) 8 . ?
O2 Y1 O3 86.81(18) 8 1_554 ?
O2 Y1 O3 86.81(18) . 1_554 ?
O2 Y1 O3 140.51(13) 14_665 1_554 ?
O2 Y1 O3 140.51(13) 11_665 1_554 ?
O6 Y1 O3 82.9(2) 8 1_554 ?
O6 Y1 O3 82.94(19) . 1_554 ?
O2 Y1 Si1 137.97(13) 8 . ?
O2 Y1 Si1 137.97(13) . . ?
O2 Y1 Si1 91.25(13) 14_665 . ?
O2 Y1 Si1 91.25(13) 11_665 . ?
O6 Y1 Si1 30.10(12) 8 . ?
O6 Y1 Si1 30.10(12) . . ?
O3 Y1 Si1 80.83(18) 1_554 . ?
O2 Y1 Y1 41.14(13) 8 11_664 ?
O2 Y1 Y1 41.14(13) . 11_664 ?
O2 Y1 Y1 91.80(13) 14_665 11_664 ?
O2 Y1 Y1 91.80(13) 11_665 11_664 ?
O6 Y1 Y1 149.79(12) 8 11_664 ?
O6 Y1 Y1 149.79(12) . 11_664 ?
O3 Y1 Y1 95.26(18) 1_554 11_664 ?
Si1 Y1 Y1 176.09(6) . 11_664 ?
O2 Y1 Y1 105.68(13) 8 11_665 ?
O2 Y1 Y1 105.68(13) . 11_665 ?
O2 Y1 Y1 39.74(14) 14_665 11_665 ?
O2 Y1 Y1 39.74(14) 11_665 11_665 ?
O6 Y1 Y1 82.74(12) 8 11_665 ?
O6 Y1 Y1 82.74(12) . 11_665 ?
O3 Y1 Y1 163.44(18) 1_554 11_665 ?
Si1 Y1 Y1 82.61(6) . 11_665 ?
Y1 Y1 Y1 101.30(4) 11_664 11_665 ?
O2 Y1 Y2 102.15(14) 8 11_664 ?
O2 Y1 Y2 37.39(12) . 11_664 ?
O2 Y1 Y2 36.14(13) 14_665 11_664 ?
O2 Y1 Y2 99.72(13) 11_665 11_664 ?
O6 Y1 Y2 91.47(12) 8 11_664 ?
O6 Y1 Y2 143.66(12) . 11_664 ?
O3 Y1 Y2 117.99(9) 1_554 11_664 ?
Si1 Y1 Y2 119.16(3) . 11_664 ?
Y1 Y1 Y2 62.67(3) 11_664 11_664 ?
Y1 Y1 Y2 70.69(2) 11_665 11_664 ?
O2 Y1 Y2 37.39(12) 8 14_664 ?
O2 Y1 Y2 102.15(14) . 14_664 ?
O2 Y1 Y2 99.72(13) 14_665 14_664 ?
O2 Y1 Y2 36.14(13) 11_665 14_664 ?
O6 Y1 Y2 143.66(12) 8 14_664 ?
O6 Y1 Y2 91.47(12) . 14_664 ?
O3 Y1 Y2 117.99(9) 1_554 14_664 ?
Si1 Y1 Y2 119.16(3) . 14_664 ?
Y1 Y1 Y2 62.67(3) 11_664 14_664 ?
Y1 Y1 Y2 70.69(2) 11_665 14_664 ?
Y2 Y1 Y2 102.15(3) 11_664 14_664 ?
O2 Y2 O6 93.86(19) 8_556 . ?
O2 Y2 O2 74.84(13) 8_556 11_665 ?
O6 Y2 O2 77.6(2) . 11_665 ?
O2 Y2 O4 88.93(19) 8_556 5_576 ?
O6 Y2 O4 97.77(19) . 5_576 ?
O2 Y2 O4 162.65(19) 11_665 5_576 ?
O2 Y2 O5 81.83(19) 8_556 14_665 ?
O6 Y2 O5 171.8(2) . 14_665 ?
O2 Y2 O5 94.42(19) 11_665 14_665 ?
O4 Y2 O5 89.18(19) 5_576 14_665 ?
O2 Y2 O5 141.71(19) 8_556 . ?
O6 Y2 O5 105.56(18) . . ?
O2 Y2 O5 77.52(19) 11_665 . ?
O4 Y2 O5 119.74(18) 5_576 . ?
O5 Y2 O5 74.40(16) 14_665 . ?
O2 Y2 O4 156.45(18) 8_556 . ?
O6 Y2 O4 75.45(18) . . ?
O2 Y2 O4 121.67(17) 11_665 . ?
O4 Y2 O4 72.21(19) 5_576 . ?
O5 Y2 O4 111.07(19) 14_665 . ?
O5 Y2 O4 61.82(17) . . ?
O2 Y2 Si2 171.07(14) 8_556 . ?
O6 Y2 Si2 85.43(14) . . ?
O2 Y2 Si2 96.34(14) 11_665 . ?
O4 Y2 Si2 99.99(13) 5_576 . ?
O5 Y2 Si2 97.73(15) 14_665 . ?
O5 Y2 Si2 31.46(13) . . ?
O4 Y2 Si2 31.38(12) . . ?
O2 Y2 Y2 104.43(14) 8_556 14_664 ?
O6 Y2 Y2 98.06(14) . 14_664 ?
O2 Y2 Y2 37.48(14) 11_665 14_664 ?
O4 Y2 Y2 158.48(13) 5_576 14_664 ?
O5 Y2 Y2 76.40(13) 14_665 14_664 ?
O5 Y2 Y2 41.21(13) . 14_664 ?
O4 Y2 Y2 97.89(11) . 14_664 ?
Si2 Y2 Y2 66.93(2) . 14_664 ?
O2 Y2 Y2 38.80(12) 8_556 14_665 ?
O6 Y2 Y2 132.42(13) . 14_665 ?
O2 Y2 Y2 89.96(14) 11_665 14_665 ?
O4 Y2 Y2 80.79(13) 5_576 14_665 ?
O5 Y2 Y2 44.30(13) 14_665 14_665 ?
O5 Y2 Y2 116.36(13) . 14_665 ?
O4 Y2 Y2 144.19(11) . 14_665 ?
Si2 Y2 Y2 141.97(5) . 14_665 ?
Y2 Y2 Y2 98.95(3) 14_664 14_665 ?
O2 Y2 Y1 38.08(13) 8_556 11_665 ?
O6 Y2 Y1 83.04(15) . 11_665 ?
O2 Y2 Y1 36.82(14) 11_665 11_665 ?
O4 Y2 Y1 126.50(13) 5_576 11_665 ?
O5 Y2 Y1 89.30(14) 14_665 11_665 ?
O5 Y2 Y1 111.15(13) . 11_665 ?
O4 Y2 Y1 153.69(12) . 11_665 ?
Si2 Y2 Y1 133.14(3) . 11_665 ?
Y2 Y2 Y1 70.03(2) 14_664 11_665 ?
Y2 Y2 Y1 62.11(2) 14_665 11_665 ?
O2 Y2 Y1 88.03(12) 8_556 . ?
O6 Y2 Y1 41.46(15) . . ?
O2 Y2 Y1 36.96(13) 11_665 . ?
O4 Y2 Y1 138.68(14) 5_576 . ?
O5 Y2 Y1 130.96(14) 14_665 . ?
O5 Y2 Y1 85.52(13) . . ?
O4 Y2 Y1 96.85(11) . . ?
Si2 Y2 Y1 85.56(3) . . ?
Y2 Y2 Y1 59.982(15) 14_664 . ?
Y2 Y2 Y1 118.93(2) 14_665 . ?
Y1 Y2 Y1 56.83(2) 11_665 . ?
O1 Zn1 O1 101.77(19) 3_775 2_576 ?
O1 Zn1 O1 101.77(19) 3_775 4_756 ?
O1 Zn1 O1 126.3(5) 2_576 4_756 ?
O1 Zn1 O1 126.3(5) 3_775 . ?
O1 Zn1 O1 101.77(19) 2_576 . ?
O1 Zn1 O1 101.77(19) 4_756 . ?
O3 Si1 O6 114.8(3) . 8 ?
O3 Si1 O6 114.8(3) . . ?
O6 Si1 O6 99.5(4) 8 . ?
O3 Si1 O1 114.5(4) . . ?
O6 Si1 O1 105.9(3) 8 . ?
O6 Si1 O1 105.9(3) . . ?
O3 Si1 Y1 132.5(3) . . ?
O6 Si1 Y1 49.8(2) 8 . ?
O6 Si1 Y1 49.8(2) . . ?
O1 Si1 Y1 113.0(3) . . ?
O3 Si1 Ba1 136.15(14) . 1_554 ?
O6 Si1 Ba1 50.6(2) 8 1_554 ?
O6 Si1 Ba1 108.7(2) . 1_554 ?
O1 Si1 Ba1 55.30(19) . 1_554 ?
Y1 Si1 Ba1 74.43(6) . 1_554 ?
O3 Si1 Ba1 136.15(14) . 2_576 ?
O6 Si1 Ba1 108.7(2) 8 2_576 ?
O6 Si1 Ba1 50.6(2) . 2_576 ?
O1 Si1 Ba1 55.30(19) . 2_576 ?
Y1 Si1 Ba1 74.43(6) . 2_576 ?
Ba1 Si1 Ba1 77.53(6) 1_554 2_576 ?
O4 Si2 O4 111.7(4) . 5_575 ?
O4 Si2 O5 111.7(3) . 5_575 ?
O4 Si2 O5 103.1(3) 5_575 5_575 ?
O4 Si2 O5 103.1(3) . . ?
O4 Si2 O5 111.7(3) 5_575 . ?
O5 Si2 O5 115.8(4) 5_575 . ?
O4 Si2 Y2 113.9(2) . 5_575 ?
O4 Si2 Y2 52.97(18) 5_575 5_575 ?
O5 Si2 Y2 52.3(2) 5_575 5_575 ?
O5 Si2 Y2 142.9(2) . 5_575 ?
O4 Si2 Y2 52.97(18) . . ?
O4 Si2 Y2 113.9(2) 5_575 . ?
O5 Si2 Y2 142.9(2) 5_575 . ?
O5 Si2 Y2 52.3(2) . . ?
Y2 Si2 Y2 159.82(10) 5_575 . ?
O4 Si2 Ba2 147.5(2) . 1_554 ?
O4 Si2 Ba2 100.34(19) 5_575 1_554 ?
O5 Si2 Ba2 53.0(2) 5_575 1_554 ?
O5 Si2 Ba2 68.5(2) . 1_554 ?
Y2 Si2 Ba2 80.75(3) 5_575 1_554 ?
Y2 Si2 Ba2 118.68(6) . 1_554 ?
O4 Si2 Ba2 100.34(19) . 5_576 ?
O4 Si2 Ba2 147.5(2) 5_575 5_576 ?
O5 Si2 Ba2 68.5(2) 5_575 5_576 ?
O5 Si2 Ba2 53.0(2) . 5_576 ?
Y2 Si2 Ba2 118.68(6) 5_575 5_576 ?
Y2 Si2 Ba2 80.75(3) . 5_576 ?
Ba2 Si2 Ba2 48.77(4) 1_554 5_576 ?
O4 Si2 Ba1 55.8(2) . 2_576 ?
O4 Si2 Ba1 55.8(2) 5_575 2_576 ?
O5 Si2 Ba1 122.1(2) 5_575 2_576 ?
O5 Si2 Ba1 122.1(2) . 2_576 ?
Y2 Si2 Ba1 79.91(5) 5_575 2_576 ?
Y2 Si2 Ba1 79.91(5) . 2_576 ?
Ba2 Si2 Ba1 155.62(2) 1_554 2_576 ?
Ba2 Si2 Ba1 155.62(2) 5_576 2_576 ?
Si1 O1 Zn1 132.9(5) . . ?
Si1 O1 Ba1 95.7(2) . 2_576 ?
Zn1 O1 Ba1 113.9(2) . 2_576 ?
Si1 O1 Ba1 95.7(2) . 1_554 ?
Zn1 O1 Ba1 113.9(2) . 1_554 ?
Ba1 O1 Ba1 98.5(2) 2_576 1_554 ?
Y2 O2 Y1 133.5(2) 8_554 . ?
Y2 O2 Y2 103.7(2) 8_554 11_664 ?
Y1 O2 Y2 105.8(2) . 11_664 ?
Y2 O2 Y1 105.8(2) 8_554 11_664 ?
Y1 O2 Y1 99.1(2) . 11_664 ?
Y2 O2 Y1 106.7(2) 11_664 11_664 ?
Si1 O3 Y1 128.3(4) . 1_556 ?
Si1 O3 Ba1 116.7(3) . . ?
Y1 O3 Ba1 96.2(2) 1_556 . ?
Si1 O3 Ba1 116.7(3) . 2_577 ?
Y1 O3 Ba1 96.2(2) 1_556 2_577 ?
Ba1 O3 Ba1 96.4(2) . 2_577 ?
Si2 O4 Y2 128.4(3) . 5_576 ?
Si2 O4 Y2 95.6(2) . . ?
Y2 O4 Y2 104.97(19) 5_576 . ?
Si2 O4 Ba1 95.6(2) . 2_576 ?
Y2 O4 Ba1 123.4(2) 5_576 2_576 ?
Y2 O4 Ba1 103.56(17) . 2_576 ?
Si2 O5 Y2 135.4(3) . 14_664 ?
Si2 O5 Y2 96.2(3) . . ?
Y2 O5 Y2 94.49(19) 14_664 . ?
Si2 O5 Ba2 97.1(2) . 5_576 ?
Y2 O5 Ba2 120.2(2) 14_664 5_576 ?
Y2 O5 Ba2 108.03(19) . 5_576 ?
Si2 O5 Ba2 81.7(2) . 1_554 ?
Y2 O5 Ba2 98.82(18) 14_664 1_554 ?
Y2 O5 Ba2 163.0(2) . 1_554 ?
Ba2 O5 Ba2 55.84(11) 5_576 1_554 ?
Si1 O6 Y2 131.2(3) . . ?
Si1 O6 Y1 100.1(3) . . ?
Y2 O6 Y1 102.1(2) . . ?
Si1 O6 Ba1 101.1(3) . 2_576 ?
Y2 O6 Ba1 116.1(2) . 2_576 ?
Y1 O6 Ba1 101.37(18) . 2_576 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O3 Si1 O1 Zn1 0.000(3) . . . . ?
O6 Si1 O1 Zn1 -127.5(2) 8 . . . ?
O6 Si1 O1 Zn1 127.5(2) . . . . ?
Y1 Si1 O1 Zn1 180.000(1) . . . . ?
Ba1 Si1 O1 Zn1 -130.40(14) 1_554 . . . ?
Ba1 Si1 O1 Zn1 130.40(14) 2_576 . . . ?
O3 Si1 O1 Ba1 -130.40(14) . . . 2_576 ?
O6 Si1 O1 Ba1 102.1(2) 8 . . 2_576 ?
O6 Si1 O1 Ba1 -2.9(3) . . . 2_576 ?
Y1 Si1 O1 Ba1 49.60(14) . . . 2_576 ?
Ba1 Si1 O1 Ba1 99.2(3) 1_554 . . 2_576 ?
O3 Si1 O1 Ba1 130.40(14) . . . 1_554 ?
O6 Si1 O1 Ba1 2.9(3) 8 . . 1_554 ?
O6 Si1 O1 Ba1 -102.1(2) . . . 1_554 ?
Y1 Si1 O1 Ba1 -49.60(14) . . . 1_554 ?
Ba1 Si1 O1 Ba1 -99.2(3) 2_576 . . 1_554 ?
O6 Si1 O3 Y1 -57.2(3) 8 . . 1_556 ?
O6 Si1 O3 Y1 57.2(3) . . . 1_556 ?
O1 Si1 O3 Y1 180.000(2) . . . 1_556 ?
Y1 Si1 O3 Y1 0.000(4) . . . 1_556 ?
Ba1 Si1 O3 Y1 -115.3(3) 1_554 . . 1_556 ?
Ba1 Si1 O3 Y1 115.3(3) 2_576 . . 1_556 ?
O6 Si1 O3 Ba1 66.3(5) 8 . . . ?
O6 Si1 O3 Ba1 -179.3(3) . . . . ?
O1 Si1 O3 Ba1 -56.5(3) . . . . ?
Y1 Si1 O3 Ba1 123.5(3) . . . . ?
Ba1 Si1 O3 Ba1 8.1(6) 1_554 . . . ?
Ba1 Si1 O3 Ba1 -121.20(12) 2_576 . . . ?
O6 Si1 O3 Ba1 179.4(3) 8 . . 2_577 ?
O6 Si1 O3 Ba1 -66.3(5) . . . 2_577 ?
O1 Si1 O3 Ba1 56.5(3) . . . 2_577 ?
Y1 Si1 O3 Ba1 -123.5(3) . . . 2_577 ?
Ba1 Si1 O3 Ba1 121.20(12) 1_554 . . 2_577 ?
Ba1 Si1 O3 Ba1 -8.1(6) 2_576 . . 2_577 ?
O4 Si2 O4 Y2 141.6(4) 5_575 . . 5_576 ?
O5 Si2 O4 Y2 26.6(5) 5_575 . . 5_576 ?
O5 Si2 O4 Y2 -98.3(4) . . . 5_576 ?
Y2 Si2 O4 Y2 83.7(3) 5_575 . . 5_576 ?
Y2 Si2 O4 Y2 -114.2(4) . . . 5_576 ?
Ba2 Si2 O4 Y2 -27.9(6) 1_554 . . 5_576 ?
Ba2 Si2 O4 Y2 -44.2(3) 5_576 . . 5_576 ?
Ba1 Si2 O4 Y2 141.6(4) 2_576 . . 5_576 ?
O4 Si2 O4 Y2 -104.3(2) 5_575 . . . ?
O5 Si2 O4 Y2 140.8(2) 5_575 . . . ?
O5 Si2 O4 Y2 15.8(3) . . . . ?
Y2 Si2 O4 Y2 -162.09(9) 5_575 . . . ?
Ba2 Si2 O4 Y2 86.3(3) 1_554 . . . ?
Ba2 Si2 O4 Y2 69.98(15) 5_576 . . . ?
Ba1 Si2 O4 Y2 -104.3(2) 2_576 . . . ?
O4 Si2 O4 Ba1 0.0 5_575 . . 2_576 ?
O5 Si2 O4 Ba1 -114.9(2) 5_575 . . 2_576 ?
O5 Si2 O4 Ba1 120.1(2) . . . 2_576 ?
Y2 Si2 O4 Ba1 -57.82(18) 5_575 . . 2_576 ?
Y2 Si2 O4 Ba1 104.3(2) . . . 2_576 ?
Ba2 Si2 O4 Ba1 -169.44(17) 1_554 . . 2_576 ?
Ba2 Si2 O4 Ba1 174.25(9) 5_576 . . 2_576 ?
O4 Si2 O5 Y2 -118.8(4) . . . 14_664 ?
O4 Si2 O5 Y2 1.3(5) 5_575 . . 14_664 ?
O5 Si2 O5 Y2 118.9(5) 5_575 . . 14_664 ?
Y2 Si2 O5 Y2 58.0(6) 5_575 . . 14_664 ?
Y2 Si2 O5 Y2 -102.8(5) . . . 14_664 ?
Ba2 Si2 O5 Y2 94.2(4) 1_554 . . 14_664 ?
Ba2 Si2 O5 Y2 148.1(5) 5_576 . . 14_664 ?
Ba1 Si2 O5 Y2 -61.1(5) 2_576 . . 14_664 ?
O4 Si2 O5 Y2 -16.0(3) . . . . ?
O4 Si2 O5 Y2 104.1(3) 5_575 . . . ?
O5 Si2 O5 Y2 -138.2(2) 5_575 . . . ?
Y2 Si2 O5 Y2 160.88(19) 5_575 . . . ?
Ba2 Si2 O5 Y2 -162.9(2) 1_554 . . . ?
Ba2 Si2 O5 Y2 -109.1(2) 5_576 . . . ?
Ba1 Si2 O5 Y2 41.8(2) 2_576 . . . ?
O4 Si2 O5 Ba2 93.2(2) . . . 5_576 ?
O4 Si2 O5 Ba2 -146.8(2) 5_575 . . 5_576 ?
O5 Si2 O5 Ba2 -29.13(7) 5_575 . . 5_576 ?
Y2 Si2 O5 Ba2 -90.0(3) 5_575 . . 5_576 ?
Y2 Si2 O5 Ba2 109.1(2) . . . 5_576 ?
Ba2 Si2 O5 Ba2 -53.84(12) 1_554 . . 5_576 ?
Ba1 Si2 O5 Ba2 150.87(7) 2_576 . . 5_576 ?
O4 Si2 O5 Ba2 147.0(2) . . . 1_554 ?
O4 Si2 O5 Ba2 -92.9(2) 5_575 . . 1_554 ?
O5 Si2 O5 Ba2 24.71(6) 5_575 . . 1_554 ?
Y2 Si2 O5 Ba2 -36.2(3) 5_575 . . 1_554 ?
Y2 Si2 O5 Ba2 162.9(2) . . . 1_554 ?
Ba2 Si2 O5 Ba2 53.84(12) 5_576 . . 1_554 ?
Ba1 Si2 O5 Ba2 -155.29(6) 2_576 . . 1_554 ?
O3 Si1 O6 Y2 -9.7(6) . . . . ?
O6 Si1 O6 Y2 113.3(4) 8 . . . ?
O1 Si1 O6 Y2 -137.1(4) . . . . ?
Y1 Si1 O6 Y2 116.0(5) . . . . ?
Ba1 Si1 O6 Y2 164.8(3) 1_554 . . . ?
Ba1 Si1 O6 Y2 -140.2(5) 2_576 . . . ?
O3 Si1 O6 Y1 -125.7(3) . . . . ?
O6 Si1 O6 Y1 -2.7(4) 8 . . . ?
O1 Si1 O6 Y1 106.9(3) . . . . ?
Ba1 Si1 O6 Y1 48.8(2) 1_554 . . . ?
Ba1 Si1 O6 Y1 103.8(2) 2_576 . . . ?
O3 Si1 O6 Ba1 130.4(3) . . . 2_576 ?
O6 Si1 O6 Ba1 -106.5(3) 8 . . 2_576 ?
O1 Si1 O6 Ba1 3.1(3) . . . 2_576 ?
Y1 Si1 O6 Ba1 -103.8(2) . . . 2_576 ?
Ba1 Si1 O6 Ba1 -55.0(2) 1_554 . . 2_576 ?

_refine_diff_density_max         2.237
_refine_diff_density_min         -1.313
_refine_diff_density_rms         0.183

